Derived from NiFe 2 O 4 for the Alkaline Hydrogen Evolution Reaction

: The development of noble-metal-free electrocatalysts is regarded as a key factor for realizing industrial-scale hydrogen production powered by renewable energy sources. Inspired by nature, which uses Fe- and Ni-containing enzymes for efﬁcient hydrogen generation, Fe/Ni-containing chalcogenides, such as oxides and sulﬁdes, received increasing attention as promising electrocatalysts to produce hydrogen. We herein present a novel synthetic procedure for mixed Fe/Ni (oxy)sulﬁde materials by the controlled (partial) sulﬁdation of NiFe 2 O 4 (NFO) nanoparticles in H 2 S-containing atmospheres. The variation in H 2 S concentration and the temperature allows for a precise control of stoichiometry and phase composition. The obtained sulﬁdized materials (NFS) catalyze the hydrogen evolution reaction (HER) with increased activity in comparison to NFO, up to − 10 and − 100 mA cm − 2 at an overpotential of approx. 250 and 450 mV, respectively. Author Contributions: Conceptualization, methodology, analysis, investigation, D.T.; writing—original writing—review K.j.P.


Introduction
The electrochemical hydrogen evolution reaction (HER) is a promising approach to foster hydrogen usage for replacing fossil fuels as major energy carriers [1,2]. Currently, electrocatalysts based on noble metals such as Pt are primarily used as cathode material in electrolyzers due to their outstanding performance; however, the scarcity of common noble metals impedes widespread application [3][4][5]. Therefore, scientists have focused on earth-abundant transition metal chalcogenides such as oxides and sulfides as cost-effective alternatives to Pt for the HER [6][7][8]. Transition metal oxides are characterized by their compositional and structural flexibility, which offer a high diversity in the electronic and crystal structure. Although transition metal oxides are regarded as catalytically inert for the HER, defect engineering or the introduction of dopants enabled an improved HER performance [9][10][11]. In contrast, transition metal sulfides can overcome the major drawbacks of metal oxides such as poor electronic conductivity, unsuitable hydrogen adsorption and limited catalytic-active sites [12][13][14]. To combine the properties of transition metal oxides and sulfides, researchers have focused on the synthesis of distinct transition metal oxysulfides, which contain oxygen and sulfur. Commonly, the synthesis of oxysulfides can be achieved by multiple pathways, including the sulfidation of an oxygenated phase, the oxidation of sulfides, the reduction of sulfates or by the co-insertion of oxygen and sulfur [15]. In this respect, Nelson et al. synthesized CoO x S y hollow nanoparticles by substituting oxide with sulfide species in CoO using ammonium sulfide in oleylamine at 100 • C [16]. The obtained electrocatalysts displayed sulfur-content-dependent HER activity, with the highest activity for CoO x S 0. 18 . Another oxysulfide material was synthesized by Sarma et al. by the anodic oxidation of WS 2 sheets [17]. Here, distinct WO x S y materials were obtained depending on the deposition potential, which has shown the highest HER performance for the WO x S y material, which was deposited at 5 V.
In terms of hydrogen production, nature has established Fe-and Ni-containing enzymes (hydrogenases), which effectively perform the reversible conversion of hydrogen to protons and electrons [18][19][20]. Inspired by the natural evolutionary choice of transition metals, numerous Fe/Ni-containing catalysts were synthesized, which showed high catalytic activities for the HER [21][22][23][24][25][26][27]. Furthermore, Fe/Ni oxysulfide materials were synthesized displaying promising activities towards the HER and oxygen evolution reaction (OER) [28,29]. However, investigating the HER activity of Fe/Ni oxysulfides with different sulfur to metal (S:M) ratios and material phases has not yet been realized.
In lieu, we herein present the synthesis of various NiFe (oxy)sulfide materials by the sulfidation of NiFe 2 O 4 with H 2 S. We demonstrate a controlled sulfidation towards a nickel containing pyrite and pyrrhotite depending on the H 2 S gas composition as well as on the temperature. Finally, we show the performance of the synthesized NiFe (oxy)sulfide materials towards the HER in an alkaline medium.

Synthesis of Sulfidized NiFe 2 O 4 (NFS) Materials
The synthesis of the starting material NiFe 2 O 4 was realized according to protocols recently published in the literature [30]. For subsequent sulfidation reactions, 100 mg of NiFe 2 O 4 was placed into a tubular furnace and purged for 10 min with H 2 S/N 2 (50:50) or H 2 S/N 2 (15:85). Maintaining the gas flow, the furnace was heated to 100 ≤ T ≤ 300 • C and the temperature was held for 1 h. The furnace was then allowed to cool down to room temperature within approx. 20 min using pressurized air while applying a N 2 gas flow.

Physical Characterization
Characterization of the investigated materials was performed by powder X-ray diffraction (PXRD) using a HUBER powder X-ray diffractometer (HUBER, Rimsting, Germany) equipped with a Mo-K α source. The 2-Θ values were converted to values from a Cu-K α , according to Bragg's law of diffraction.
The particle sizes of the synthesized electrocatalysts were determined using a SALD-2300 laser diffraction particle size analyzer (Shimadzu, Duisburg, Germany) equipped with a SALD-BC23 batch cell. The respective samples were prepared by dispersing approx. 10 mg of the catalyst material for 1 min in 1 mL isopropyl alcohol using an ultra-sonic bath. Subsequently, a portion of the dispersion was added to the batch cell, which was filled with isopropyl alcohol. The obtained particle sizes were calculated using the Fraunhofer approximation and the volume was chosen based on the dimensions of the particle amount.
A Gemini2 Merlin HR-FESEM (ZEISS, Oberkochen, Germany) was used for scanning electron microscopy (SEM), equipped with an OXFORD AZtecEnergy X-ray microanalysis system for energy dispersive X-ray spectroscopy (EDX). Samples were dispersed in 1 mL isopropyl alcohol and ultra-sonicated for 1 min. Afterwards, the samples were drop-casted on a flat Si Wafer for analysis. The SEM images were recorded at an acceleration voltage of 5 kV while EDX mappings were performed from 0-20 kV.
X-ray photoelectron spectroscopy (XPS) measurements were performed with a polychromatic Al-K α X-ray source (anode operating at 14 kV and 13 mA) combined with an ultra−High-vacuum (UHV, 10 −9 mbar) setup and a hemispherical analyzer (type CLAM2, VG, Scientific, Thermo Fisher Scientific, Dreieich, Germany). A pass energy of 100 eV was applied to record the spectra.

Electrochemical Characterization
The (oxy)sulfide electrocatalysts were investigated as drop-casted materials on a glassy carbon (GC) rod electrode. For this purpose, 11.78 mg of the catalyst material was dispersed in a mixture composed of 0.30 mL water, 0.15 mL isopropanol and 0.05 mL Nafion (5 % in aliphatic alcohols) using an ultra-sonic bath for 30 min. Subsequently, 3 µL of the catalyst ink was applied on a GC electrode (d = 3 mm, 1 mg cm −2 catalyst), which was dried at room temperature for 30 min. Before drop-casting, the GC electrode was polished using Al 2 O 3 pastes with grain sizes of 0.30 and 0.05 µm for 3 min, each followed by ultra-sonication in Milli-Q water for 5 min.
Electrochemical measurements were performed in a three-electrode setup, employing the catalyst-modified GC working electrode (WE), a Pt mesh counter electrode (CE) and a Hg/HgO (1 M KOH) reference electrode (RE) in 1 M KOH. The WE and CE were separated by utilizing an H-type electrolysis cell with both half-cells being separated by an anion exchange separator (Zirfon ® , AGFA, Mortsel, The Netherlands). Electrochemical measurements were conducted using a GAMRY Reference 600 or Reference 600 + (C3-Analysentechnik, Haar, Germany) and the measured potentials were converted to the reversible hydrogen electrode (RHE) reference according to the equation: For the HER experiments, the material was first electrochemically conditioned through cyclic voltammetry (CV) between 0 and −0.3 V vs. RHE at 100 mV s −1 until a stable voltammogram was obtained. The investigation of the electrochemical surface area (ECSA) was realized through CV measurements between −0.16 and −0.24 V vs. RHE at scan rates of 40, 80, 120, 160 and 200 mV s −1 , respectively. Changes in the electrochemical activity were monitored via linear sweep voltammetry (LSV) between 0 and −0.45 V vs. RHE at a scan rate of 1 mV s −1 . Electrochemical impedance spectroscopy (EIS) measurements were conducted at −0.4 V vs. RHE from 100 kHz to 0.10 Hz taking 7 points per decade at an amplitude of 7 mV rms. Stability tests were performed using chronopotentiometry at −10 or −100 mA cm −2 for at least one hour.

Synthesis and Physical Characterization
The synthesis of NiFe-(oxy)sulfides (NFS) was performed by utilizing NiFe 2 O 4 (NFO) as the starting compound. The NFO precursor was treated with different H 2 S gas compositions (H 2 S/N 2 , (50:50) and H 2 S/H 2 (15:85)) at different temperatures (100 ≤ T ≤ 300 • C) to control the sulfur to metal (S:M) ratio in the materials [31]. For clarity, the synthesized materials are referred to as NFS T −N 2 and NFS T −H 2 , where T represents the temperature in • C and N 2 and H 2 the diluting gases.
The obtained materials were analyzed by powder X-ray diffraction (PXRD) and show distinct phase formations depending on the applied temperature and H 2 S gas composition ( Figure 1). Treatment of NiFe 2 O 4 in either the H 2 S/N 2 or H 2 S/H 2 gas mixture results in no visible change in the powder pattern compared to NFO when heated below 200 • C, indicating a conservation of the NFO phase. Starting at 200 • C, phase transformations occur, which become more prominent at higher temperatures. Using a H 2 S/N 2 atmosphere, phase transformations towards nickelian pyrite (Ni 0.35 Fe 0.65 S 2 ) were observed, while the usage of H 2 S/H 2 resulted in phase transformations towards nickelian pyrrhotite (Ni 0.35 Fe 0.65 S). Notably, the crystallinity of the synthesized materials increases with temperature and no further phase transformation occurred after heating the samples for longer than 1 h. temperature and no further phase transformation occurred after heating the samples for longer than 1 h.
To further clarify the composition of the obtained NFS materials, X-ray photoelectron spectroscopy (XPS) measurements were performed ( Figure S1 in Supplementary Materials). The XPS spectra show characteristic peaks of the two p3/2 orbitals of Ni and Fe at approx. 858 and 710 eV, respectively. Furthermore, all materials show a peak in the O 1s spectrum at approx. 532 eV, which can be ascribed to either metal-oxygen bonds, lowcoordinated oxygen ions at the surface or adsorbed water [29]. Interestingly, the XPS analysis reveals the presence of sulfur in each NFS sample, which indicates a sulfidation of NFO below 200 °C.
In order to quantify the S:M ratios, the synthesized materials were subjected to energy dispersive spectroscopy (EDX) ( Table 1). While no phase changes in the powder patterns are observable, sulfur was detected in the NFS100−N2 and NFS100−H2 materials with S:M ratios of 1.09 ± 0.09 and 0.79 ± 0.26, respectively. For NFS−N2, the S:M ratio undergoes a slight increase until 250 °C (S:M ratio = 1.49 ± 0.06) and a much steeper increase up to 300 °C with a S:M ratio of 1.98 ± 0.26. For the NFS−H2 materials, the S:M ratio increases until reaching a S:M ratio of 1.20 ± 0.08 for NFS200−H2, which subsequently decreases to a S:M ratio of 1.15 ± 0.06 for NFS300−H2. According to the EDX analysis, the sum formulas of the nickelian pyrite and pyrrhotite were calculated to Ni0.30Fe0.71S1.99 and Ni0.30Fe0.64S1.06, at that point reaching complete sulfidation. Thus, the obtainable phases (NFO, nickelian pyrite or pyrrhotite) as well as the degree of sulfidation can be controlled by the variation of S-source gas composition and temperature.  To further clarify the composition of the obtained NFS materials, X-ray photoelectron spectroscopy (XPS) measurements were performed ( Figure S1 in Supplementary Materials). The XPS spectra show characteristic peaks of the two p 3/2 orbitals of Ni and Fe at approx. 858 and 710 eV, respectively. Furthermore, all materials show a peak in the O 1s spectrum at approx. 532 eV, which can be ascribed to either metal-oxygen bonds, low-coordinated oxygen ions at the surface or adsorbed water [29]. Interestingly, the XPS analysis reveals the presence of sulfur in each NFS sample, which indicates a sulfidation of NFO below 200 • C.
In order to quantify the S:M ratios, the synthesized materials were subjected to energy dispersive spectroscopy (EDX) ( Table 1)  Scanning electron microscopy (SEM) characterization of the obtained materials reveals comparable particle morphologies and sizes for all tested samples (Figures S2 and S3). In general, spherical shaped particles with sizes in the nanometer range are present, which form larger agglomerates with a rough surface morphology. A more detailed picture of the size distribution of the obtained NFS materials is given by laser diffraction analysis ( Figure S4). In general, all materials display a broad particle size distribution. For example, the NFO precursor shows a significant number of particles in the nanometer range as well as in the micrometer range (up to 100 µm). In comparison, the particle size distribution of the NFS materials shows a shift towards larger particles of up to 400 µm, indicating agglomeration. However, a correlation of the particle sizes with the applied temperature cannot be observed and for obtaining smaller particle sizes post-synthetic milling is suggested.

Electrochemical Hydrogen Evolution Reaction
To further investigate the dependence of the alkaline HER activity on the S:M ratio of the synthesized NFS compounds and to observe trends arising from this alteration, electrodes were prepared via drop-casting and served as working electrodes in a threeelectrode setup employing an H-type electrolysis cell.
For a first analysis, the electrochemical activity was determined by linear sweep voltammetry (LSV) at a scan rate of 1 mV s −1 (Figure 2a,d). The investigated electrocatalytic materials display distinct overpotentials vs. RHE at a current density of −10 mA cm −2 depending on the catalyst composition. For instance, the usage of the NFO precursor as an HER catalyst resulted in almost no catalytic activity. In contrast, all sulfidized materials show a lower overpotential compared to NFO. Using the NFS−N 2 electrocatalysts, the lowest overpotential at −10 mA cm −2 was observed for NFS 100 −N 2 at 266 ± 12 mV. The overpotential increases for catalysts synthesized at higher temperatures up to 394 ± 24 mV for NFS 250 −N 2 . Surprisingly, the NFS 300 −N 2 electrocatalyst displays an increased catalytic activity in contrast to NFS 250 −N 2 with an overpotential of 346 ± 4 mV. In comparison, the highest HER activity for the NFS−H 2 electrocatalysts was observed for NFS 250 −H 2 with an overpotential of 302 ± 9 mV, which increases to 408 ± 30 mV for NFS 150 −H 2 . Notably, the lowest overpotentials are observed for NFS−N 2 electrocatalysts synthesized at temperatures around 100 • C and for NFS−H 2 electrocatalysts synthesized around 250 • C, which show a S:M ratio of approx. 1:1. However, since most of the NFS−H 2 electrocatalysts display similar S:M ratios, the presence of the nickelian pyrrhotite phase seems to play a major role for increased HER activity.
To test this theory, we normalized the LSV curves by the electrochemical surface area (ECSA) to exclude particle size effects from the electrochemical activity. For this purpose, the ECSA was determined by measuring the double layer capacitance (C DL ) of the materials using cyclic voltammetry (Figure 2b,e). The NFS−N 2 electrocatalysts display similar C DL values, with NFS 150 −N 2 having the highest C DL of 51 ± 6 mF cm −2 , followed by NFS 250 −N 2 (49 ± 2 mF cm −2 ), NFS 200 −N 2 (45 ± 5 mF cm −2 ) and NFS 100 −N 2 (44 ± 3 mF cm −2 ). Interestingly, the NFS 300 −N 2 electrocatalyst displays a C DL of 11 ± 1 mF cm −2 , which is several times lower than the other NFS−N 2 electrocatalysts. The NFS−H 2 electrocatalysts display the highest C DL for NFS 100 −H 2 (44 ± 3 mF cm −2 ) and NFS 150 −H 2 (51 ± 6 mF cm −2 ), which decreases with increasing temperature during the synthesis down to 12 ± 2 mF cm −2 for NFS 300 −H 2 . The calculation of the ECSA was performed by dividing the obtained C DL values by a specific capacitance C S of 0.04 mF cm −2 [35]. The overpotentials from the LSV curves normalized to the ECSA were obtained at a current density of 0.02 mA cm −2 ECSA (Figure 2c,f). Here, the ECSA normalization for the NFS−N 2 electrocatalysts results in clearly separated overpotentials for NFS 100 −N 2 (329 ± 13 mV) and the NFS 150 −N 2 (353 ± 21 mV) electrocatalysts, which have shown similar low non−Normalized overpotentials. A similar trend can be observed for NFS 250 −H 2 and NFS 300 −H 2 catalyzing the HER with overpotentials of 300 ± 9 mV and 272 ± 9 mV, respectively. Notably, NFS 100 −N 2 catalyzes the HER at the lowest non−Normalized overpotential, while NFS 300 −H 2 displays the lowest normalized overpotential. Thus, consideration of particle size effects on the Energies 2022, 15, 543 6 of 9 electrocatalytic activity is important to determine intrinsic material properties. In addition, we performed electrochemical impedance spectroscopy (EIS) measurements, which reveal similar trends compared to the non−Normalized LSV data ( Figure S5)  To test this theory, we normalized the LSV curves by the electrochemical surface area (ECSA) to exclude particle size effects from the electrochemical activity. For this purpose, the ECSA was determined by measuring the double layer capacitance (CDL) of the materials using cyclic voltammetry (Figure 2b,e). The NFS−N2 electrocatalysts display similar CDL values, with NFS150−N2 having the highest CDL of 51 ± 6 mF cm −2 , followed by NFS250−N2 (49 ± 2 mF cm −2 ), NFS200−N2 (45 ± 5 mF cm −2 ) and NFS100−N2 (44 ± 3 mF cm −2 ). Interestingly, the NFS300−N2 electrocatalyst displays a CDL of 11 ± 1 mF cm −2 , which is several times lower than the other NFS−N2 electrocatalysts. The NFS−H2 electrocatalysts display the highest CDL for NFS100−H2 (44 ± 3 mF cm -2 ) and NFS150−H2 (51 ± 6 mF cm −2 ), which decreases with increasing temperature during the synthesis down to 12 ± 2 mF cm −2 for NFS300−H2. The calculation of the ECSA was performed by dividing the obtained CDL values by a specific capacitance CS of 0.04 mF cm −2 [35]. The overpotentials from the LSV curves normalized to the ECSA were obtained at a current density of 0.02 mA cm −2 ECSA (Figure 2c,f). Here, the ECSA normalization for the NFS−N2 electrocatalysts results in clearly separated overpotentials for NFS100−N2 (329 ± 13 mV) and the NFS150−N2 (353 ± 21 mV) electrocatalysts, which have shown similar low non−Normalized overpotentials. A similar trend can be observed for NFS250−H2 and NFS300−H2 catalyzing the HER with overpotentials of 300 ± 9 mV and 272 ± 9 mV, respectively. Notably, NFS100−N2 catalyzes the HER at the lowest non−Normalized overpotential, while NFS300−H2 displays the lowest normalized overpotential. Thus, consideration of particle size effects on the electrocatalytic activity is important to determine intrinsic material properties. In addition, we performed electrochemical impedance spectroscopy (EIS) measurements, which reveal similar trends compared to the non−Normalized LSV data ( Figure S5). Here, To test the stability of the NFS electrocatalysts, we performed chronopotentiometry experiments for 1 h at a current density of −10 mA cm −2 (Figure 3a,b). A stable performance with a minor activation or deactivation behavior can be observed depending on the investigated electrocatalyst. For example, the NFO precursor catalyst shows the highest potential required to catalyze the HER and shows an activation behavior over the duration of the experiment. However, the overall activity after 1 h is inferior to the synthesized NFS materials. In comparison, most of the NFS−N 2 electrocatalysts, except for NFS 250 −N 2 , show a slight deactivation within 1 h. The deactivation behavior can also be observed for NFS 100 −H 2 and NFS 200 −H 2 ; however, a deactivation behavior from a particle detachment from the electrode cannot be generally excluded. Interestingly, NFS 250 −H 2 and NFS 300 −H 2 , which catalyze the HER with the lowest potential, show a stable performance. We therefore subjected the NFS 300 −H 2 electrocatalyst to an elongated electrolysis at −10 and −100 mA cm −2 for 10 h, respectively (Figure 3c). Here, the HER was also catalyzed with a stable performance by NFS 300 −H 2 .
Energies 2022, 15, 543 7 of 9 Energies 2022, 15, x FOR PEER REVIEW therefore subjected the NFS300−H2 electrocatalyst to an elongated electrolysis at −1 −100 mA cm −2 for 10 h, respectively (Figure 3c). Here, the HER was also catalyzed stable performance by NFS300−H2. It can be concluded that NiFe (oxy)sulfide materials catalyze the electrochemica with efficiencies depending on the S:M ratio and the materials phase. The NFS100−N NFSH2,300 °C show high overall activities; however, since the NFS−N2 materials mostl to deactivate during catalysis, the usage of the fully sulfidized NFS300−H2 material s be prioritized, which displayed stability for 10 h at −100 mA cm −2 .

Conclusions
A series of bimetallic NiFe (oxy)sulfide materials was synthesized by heatin transition metal oxide NFO in H2S-containing atmospheres. Depending on the cho the H2S gas composition and the applied reaction temperature, a control of the incorporation into NFO and the materials phase was achieved. For example, a sulfi of NFO was observed at low temperatures of 100 °C and full conversion into the nic pyrite (Ni0.30Fe0.71S1.99) and pyrrhotite (Ni0.30Fe0.64S1.06) sulfide materials were reali 300 °C. SEM analysis and the particle size analysis by the laser diffraction tech revealed a broad particle size distribution caused by the particle sintering of th materials.
Furthermore, we assessed the electrochemical HER performance of the NFS ma in 1 M KOH. The electrochemical performance varied with the sulfur content an materials phase. Materials with a S:M ratio of approx. 1 and/or a nickelian pyrr phase catalyzed the HER with the lowest overpotentials of 266 ± 12 mV and 302 ± vs. RHE at −10 mA cm −2 for NFS100−N2 and NFS250−H2, respectively. Additiona normalization of the geometric current density by the ECSA was performed, revealed the lowest overpotential of 272 ± 9 mV vs. RHE at a current density of 0.0 cm −2 ECSA catalyzed by NFS300−H2. Here, NFS100−N2 and NFS300−H2 showed the l overpotential for the non−Normalized and the ECSA−Normalized LSV data, respec Therefore, particle size effects should be included in the consideration of the HER ac Finally, preliminary stability measurements have revealed a rather deactivating beh of NFS−N2 materials, while the NFS300−H2 was able to catalyze the HER at current de of −10 and −100 mA cm −2 with stable potentials for 10 h.
These results represent another step towards designing transition metal chalcog catalyst materials for the electrochemical HER and point the way towards the efficient stoichiometric formulations of NiFe (oxy)sulfide-based catalysts.  Figure S2: Deconvoluted XPS spectra of NFS Figure S3: Deconvoluted XPS spectra of NFS100−N2. Figure S4: SEM images of the synth NFS−N2 materials. Figure   It can be concluded that NiFe (oxy)sulfide materials catalyze the electrochemical HER with efficiencies depending on the S:M ratio and the materials phase. The NFS 100 −N 2 and NFS H2,300 • C show high overall activities; however, since the NFS−N 2 materials mostly tend to deactivate during catalysis, the usage of the fully sulfidized NFS 300 −H 2 material should be prioritized, which displayed stability for 10 h at −100 mA cm −2 .

Conclusions
A series of bimetallic NiFe (oxy)sulfide materials was synthesized by heating the transition metal oxide NFO in H 2 S-containing atmospheres. Depending on the choice of the H 2 S gas composition and the applied reaction temperature, a control of the sulfur incorporation into NFO and the materials phase was achieved. For example, a sulfidation of NFO was observed at low temperatures of 100 • C and full conversion into the nickelian pyrite (Ni 0.30 Fe 0.71 S 1.99 ) and pyrrhotite (Ni 0.30 Fe 0.64 S 1.06 ) sulfide materials were realized at 300 • C. SEM analysis and the particle size analysis by the laser diffraction technique revealed a broad particle size distribution caused by the particle sintering of the NFS materials.
Furthermore, we assessed the electrochemical HER performance of the NFS materials in 1 M KOH. The electrochemical performance varied with the sulfur content and the materials phase. Materials with a S:M ratio of approx. 1 and/or a nickelian pyrrhotite phase catalyzed the HER with the lowest overpotentials of 266 ± 12 mV and 302 ± 9 mV vs. RHE at −10 mA cm −2 for NFS 100 −N 2 and NFS 250 −H 2 , respectively. Additionally, a normalization of the geometric current density by the ECSA was performed, which revealed the lowest overpotential of 272 ± 9 mV vs. RHE at a current density of 0.02 mA cm −2 ECSA catalyzed by NFS 300 −H 2 . Here, NFS 100 −N 2 and NFS 300 −H 2 showed the lowest overpotential for the non−Normalized and the ECSA−Normalized LSV data, respectively. Therefore, particle size effects should be included in the consideration of the HER activity. Finally, preliminary stability measurements have revealed a rather deactivating behavior of NFS−N 2 materials, while the NFS 300 −H 2 was able to catalyze the HER at current densities of −10 and −100 mA cm −2 with stable potentials for 10 h.
These results represent another step towards designing transition metal chalcogenide catalyst materials for the electrochemical HER and point the way towards the most efficient stoichiometric formulations of NiFe (oxy)sulfide-based catalysts.
Supplementary Materials: The following are available online at https://www.mdpi.com/article/10 .3390/en15020543/s1, Figure S1: XPS data of the synthesized NFS materials. Figure S2: Deconvoluted XPS spectra of NFS 300 −H 2 . Figure S3: Deconvoluted XPS spectra of NFS 100 −N 2 . Figure S4: SEM images of the synthesized NFS−N 2 materials. Figure S5: SEM images of the synthesized NFS−H 2 materials. Figure S6: Representative SEM images at NFS 100 −H 2 and NFS 100 −N 2 at distinct magnifications. Figure S7: Particle size analysis by laser diffraction. Figure S8: Representative CV measurements for determination of C DL . Figure S9: EIS spectra of the NFS materials. Figure S10: Tafel analysis of NFS materials.